advertisement

CHAPTER 9 PHASE DIAGRAMS PROBLEM SOLUTIONS 9.24 (a) We are given that the mass fractions of and liquid phases are both 0.5 for a 40 wt% Pb-60 wt% Mg alloy and asked to estimate the temperature of the alloy. Using the appropriate phase diagram, Figure 9.18, by trial and error with a ruler, a tie line within the + L phase region that is divided in half for an alloy of this composition exists at about 540C. (b) We are now asked to determine the compositions of the two phases. This is accomplished by noting the intersections of this tie line with both the solidus and liquidus lines. intersections, C = 26 wt% Pb, and C = 54 wt% Pb. L 9.35 We are given a hypothetical eutectic phase diagram for which C From these = 64 wt% B, C = 12 wt% B at the eutectic temperature, and also that W = 0.367 and W = 0.768; from this we are asked to ' determine the composition of the alloy. Let us write lever rule expressions for W and W ' W = W' = C o C C C = Co 12 C 12 eutectic = 0.768 C o C eutectic C 64 = o = 0.367 C Ceutectic C 64 Thus, we have two simultaneous equations with C o and C as unknowns. Solving them for C o gives C = 75 wt% B. o 9.41 In this problem we are asked to specify temperature-composition points for all eutectics, eutectoids, peritectics, and congruent phase transformations for the tin-gold system. There are two eutectics on this phase diagram. One exists at 10 wt% Au-90 wt% Sn and 217C. The reaction upon cooling is L + The other eutectic exists at 80 wt% Au-20 wt% Sn and 280C. This reaction upon cooling is 239 L + There are three peritectics. One exists at 30 wt% Au-70 wt% Sn and 252C. Its reaction upon cooling is as follows: L + The second peritectic exists at 45 wt% Au-55 wt% Sn and 309C. This reaction upon cooling is L + The third peritectic exists at 92 wt% Au-8 wt% Sn and 490C. This reaction upon cooling is L + There is one congruent melting point at 62.5 wt% Au-37.5 wt% Sn and 418C. Its reaction upon cooling is L No eutectoids are present. 9.45 Below is shown the phase diagram for these two A and B metals. 240 9.54 We are called upon to consider various aspects of 2.5 kg of austenite containing 0.65 wt% C, that is cooled to below the eutectoid. (a) Ferrite is the proeutectoid phase since 0.65 wt% C is less than 0.76 wt% C. (b) For this portion of the problem, we are asked to determine how much total ferrite and cementite form. Application of the appropriate lever rule expression yields W = CFe C C o 3 CFe C C 3 = 6.70 0.65 = 0.91 6.70 0.022 which corresponds to (0.91)(2.5 kg) = 2.26 kg of total ferrite. Similarly, for total cementite, Co C 0.65 0.022 WFe C = = = 0.09 CFe C C 6.70 0.022 3 3 Or (0.09)(2.5 kg) = 0.24 kg of total cementite form. (c) Now consider the amounts of pearlite and proeutectoid ferrite. Using Equation (9.18) Wp = C o' 0.022 0.74 = 0.65 0.022 = 0.85 0.74 241 This corresponds to (0.85)(2.5 kg) = 2.12 kg of pearlite. Also, from Equation (9.19), W' = 0.76 0.65 = 0.15 0.74 Or, there are (0.15)(2.5 kg) = 0.38 kg of proeutectoid ferrite. (d) Schematically, the microstructure would appear as: 9.56 This problem asks that we determine the carbon concentration in an iron-carbon alloy, given the mass fractions of proeutectoid ferrite and pearlite (0.286 and 0.714, respectively). From Equation (9.18) Wp = 0.714 = Co' 0.022 which yields C 'o = 0.55 wt% C. 242 0.74